#------------------------------------------------------------------------------
#$Date: 2019-11-17 15:32:33 +0200 (Sun, 17 Nov 2019) $
#$Revision: 230902 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/14/7231405.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7231405
loop_
_publ_author_name
'Collings, Ines E.'
'Manna, Rudra Sekhar'
'Tsirlin, Alexander A.'
'Bykov, Maxim'
'Bykova, Elena'
'Hanfland, Michael'
'Gegenwart, Philipp'
'van Smaalen, Sander'
'Dubrovinsky, Leonid'
'Dubrovinskaia, Natalia'
_publ_section_title
;
 Pressure dependence of spin canting in ammonium metal formate
 antiferromagnets.
;
_journal_issue                   37
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              24465
_journal_page_last               24476
_journal_paper_doi               10.1039/c8cp03761b
_journal_volume                  20
_journal_year                    2018
_chemical_formula_moiety         'C6 H6 Mn2 O12, N2 H8'
_chemical_formula_sum            'C6 H14 Mn2 N2 O12'
_chemical_formula_weight         416
_space_group_IT_number           4
_space_group_name_Hall           'P 2yb'
_space_group_name_H-M_alt        'P 1 21 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_audit_creation_method           'Jana2006 Version : 25/10/2015'
_audit_update_record
;
2018-08-09 deposited with the CCDC.
2018-08-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 89.99(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.714(5)
_cell_length_b                   7.119(4)
_cell_length_c                   14.031(5)
_cell_measurement_reflns_used    132
_cell_measurement_temperature    293
_cell_measurement_theta_max      10.97
_cell_measurement_theta_min      1.95
_cell_volume                     670.6(7)
_computing_cell_refinement       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.46 (Rigaku OD, 2015)'
_diffrn_ambient_pressure         '1.38 GPa'
_diffrn_ambient_temperature      293
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.84
_diffrn_measured_fraction_theta_max 0.82
_diffrn_measurement_device       'ID15B beamline, ESRF'
_diffrn_measurement_device_type
'esperanto-CrysAlisPro-abstract goniometer imported esperanto images'
_diffrn_measurement_method       'ω scans'
_diffrn_measurement_specimen_support 'diamond-anvil cell'
_diffrn_radiation_monochromator  synchrotron
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.41111
_diffrn_reflns_av_R_equivalents  0.0421
_diffrn_reflns_av_unetI/netI     0.0982
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            1974
_diffrn_reflns_theta_full        10.18
_diffrn_reflns_theta_max         11.9
_diffrn_reflns_theta_min         1.68
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    0.418
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.381
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.46 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.0604
_exptl_crystal_description       'hexagonal bipyramid'
_exptl_crystal_F_000             404
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.050
_refine_diff_density_max         1.30
_refine_diff_density_min         -1.20
_refine_ls_abs_structure_details
'  714 of Friedel pairs used in the refinement'
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    3.74
_refine_ls_goodness_of_fit_ref   2.97
_refine_ls_hydrogen_treatment    constr
_refine_ls_number_constraints    49
_refine_ls_number_parameters     87
_refine_ls_number_reflns         1974
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1952
_refine_ls_R_factor_gt           0.1402
_refine_ls_shift/su_max          0.0167
_refine_ls_shift/su_mean         0.0020
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1499
_refine_ls_wR_factor_ref         0.1631
_reflns_number_gt                1076
_reflns_number_total             1974
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            c8cp03761b2.cif
_cod_data_source_block           AMnF_c2_p01
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7231402--7231432.cif.
;
_cod_database_code               7231405
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,y+1/2,-z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
Mn1 Mn 0.6340(7) 0.7078(8) 0.8501(3) Uani 0.0488(13) 2 1 d
Mn2 Mn 0.1336(7) 0.2202(8) 0.6501(3) Uani 0.0488(13) 2 1 d
C1 C 0.906(5) -0.138(6) 0.551(2) Uiso 0.078(5) 2 1 d
C2 C 0.523(6) 1.014(6) 0.705(3) Uiso 0.078(5) 2 1 d
C3 C 1.019(5) 0.913(5) 0.801(2) Uiso 0.057(4) 2 1 d
C4 C 0.253(5) 0.473(5) 0.816(2) Uiso 0.063(4) 2 1 d
C5 C 0.762(5) 0.423(4) 0.6920(18) Uiso 0.052(4) 2 1 d
C6 C 0.616(5) 0.583(5) 1.040(2) Uiso 0.056(4) 2 1 d
O1 O 1.069(3) 1.075(3) 0.7819(13) Uiso 0.057(4) 2 1 d
O2 O 0.488(3) 0.948(3) 0.9280(13) Uiso 0.056(4) 2 1 d
O3 O 0.362(3) 0.576(4) 0.8644(14) Uiso 0.063(4) 2 1 d
O4 O 0.729(3) 0.596(3) 0.9835(13) Uiso 0.056(4) 2 1 d
O5 O 0.776(3) 0.474(3) 0.7700(13) Uiso 0.052(4) 2 1 d
O6 O 0.419(4) 1.087(4) 0.6337(16) Uiso 0.078(5) 2 1 d
O7 O 0.912(3) 0.854(3) 0.8574(13) Uiso 0.057(4) 2 1 d
O8 O 0.276(3) 0.452(3) 0.7297(13) Uiso 0.063(4) 2 1 d
O9 O 0.842(3) 0.333(3) 0.6328(13) Uiso 0.052(4) 2 1 d
O10 O 0.986(4) 0.018(4) 0.5663(16) Uiso 0.078(5) 2 1 d
O11 O 0.570(4) 0.861(4) 0.7182(16) Uiso 0.078(5) 2 1 d
O12 O 0.235(4) 0.352(4) 0.5122(15) Uiso 0.078(5) 2 1 d
N1 N 0.637(3) 0.213(5) 0.4741(15) Uani 0.061(8) 2 1 d
N2 N 0.117(3) 0.708(5) 1.0230(15) Uani 0.061(8) 2 1 d
H1c1 H 0.948229 -0.248111 0.585849 Uiso 0.0932 2 1 d
H1c2 H 0.565061 1.101996 0.753067 Uiso 0.0937 2 1 d
H1c6 H 0.590086 0.699329 1.072711 Uiso 0.0672 2 1 d
H1c5 H 0.638901 0.469569 0.666221 Uiso 0.062 2 1 d
H1c3 H 1.080374 0.818581 0.761125 Uiso 0.069 2 1 d
H1c4 H 0.146152 0.406806 0.847244 Uiso 0.0756 2 1 d
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C -0.0001 0.0005 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
H 0.0000 0.0000 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.1790 0.2615 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
N 0.0006 0.0010 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0018 0.0018 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O2 Mn1 O3 . . 85.0(9)
O2 Mn1 O4 . . 89.4(8)
O2 Mn1 O5 . . 178.6(7)
O2 Mn1 O7 . . 89.3(8)
O2 Mn1 O11 . . 86.9(9)
O3 Mn1 O4 . . 90.6(8)
O3 Mn1 O5 . . 95.1(9)
O3 Mn1 O7 . . 171.5(8)
O3 Mn1 O11 . . 97.8(9)
O4 Mn1 O5 . . 92.0(8)
O4 Mn1 O7 . . 83.0(8)
O4 Mn1 O11 . . 170.5(9)
O5 Mn1 O7 . . 90.8(8)
O5 Mn1 O11 . . 91.7(8)
O7 Mn1 O11 . . 88.1(9)
O1 Mn2 O6 1_445 1_545 93.4(9)
O1 Mn2 O8 1_445 . 90.7(8)
O1 Mn2 O9 1_445 1_455 95.4(8)
O1 Mn2 O10 1_445 1_455 93.2(9)
O1 Mn2 O12 1_445 . 173.1(9)
O6 Mn2 O8 1_545 . 89.8(9)
O6 Mn2 O9 1_545 1_455 166.8(8)
O6 Mn2 O10 1_545 1_455 93.4(10)
O6 Mn2 O12 1_545 . 79.8(9)
O8 Mn2 O9 . 1_455 99.9(8)
O8 Mn2 O10 . 1_455 174.8(9)
O8 Mn2 O12 . . 89.5(8)
O9 Mn2 O10 1_455 1_455 76.3(9)
O9 Mn2 O12 1_455 . 91.3(8)
O10 Mn2 O12 1_455 . 87.0(9)
O10 C1 O12 . 2_646 118(3)
O10 C1 H1c1 . . 120.99
O12 C1 H1c1 2_646 . 120.99
O6 C2 O11 . . 130(4)
O6 C2 H1c2 . . 115.23
O11 C2 H1c2 . . 115.23
O1 C3 O7 . . 131(3)
O1 C3 H1c3 . . 114.53
O7 C3 H1c3 . . 114.53
O3 C4 O8 . . 122(3)
O3 C4 H1c4 . . 118.95
O8 C4 H1c4 . . 118.95
O5 C5 O9 . . 143(3)
O5 C5 H1c5 . . 108.5
O9 C5 H1c5 . . 108.5
O2 C6 O4 2_647 . 134(3)
O2 C6 H1c6 2_647 . 113.1
O4 C6 H1c6 . . 113.1
Mn2 O1 C3 1_665 . 133.3(19)
Mn1 O2 C6 . 2_657 169.9(19)
Mn1 O3 C4 . . 138(2)
Mn1 O4 C6 . . 117(2)
Mn1 O5 C5 . . 133(2)
Mn2 O6 C2 1_565 . 124(2)
Mn1 O7 C3 . . 133(2)
Mn2 O8 C4 . . 122(2)
Mn2 O9 C5 1_655 . 123.2(19)
Mn2 O10 C1 1_655 . 154(2)
Mn1 O11 C2 . . 131(3)
Mn2 O12 C1 . 2_656 113(2)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Mn1 O2 . 2.25(2)
Mn1 O3 . 2.06(2)
Mn1 O4 . 2.13(2)
Mn1 O5 . 2.22(2)
Mn1 O7 . 2.14(2)
Mn1 O11 . 2.19(2)
Mn2 O1 1_445 2.16(2)
Mn2 O6 1_545 2.15(3)
Mn2 O8 . 2.21(2)
Mn2 O9 1_455 2.13(2)
Mn2 O10 1_455 2.11(3)
Mn2 O12 . 2.25(2)
C1 O10 . 1.25(5)
C1 O12 2_646 1.31(4)
C1 H1c1 . 0.96
C2 O6 . 1.33(4)
C2 O11 . 1.15(5)
C2 H1c2 . 0.96
C3 O1 . 1.23(4)
C3 O7 . 1.15(4)
C3 H1c3 . 0.96
C4 O3 . 1.24(4)
C4 O8 . 1.23(3)
C4 H1c4 . 0.96
C5 O5 . 1.16(3)
C5 O9 . 1.18(3)
C5 H1c5 . 0.96
C6 O2 2_647 1.26(4)
C6 O4 . 1.11(4)
C6 H1c6 . 0.96
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
1 0.264(6) 1 0 0 0 1 0 0 0 1
2 0.301(4) 0.991 0 -0.2787 0 -1 0 -0.064 0 -0.991
3 0.435(4) -0.611 0 -1.6542 0 -1 0 -0.3787 0 0.6113
